- Nano Review
- Open Access
Enhancement of the photoelectric performance of dye-sensitized solar cells using Ag-doped TiO2 nanofibers in a TiO2 film as electrode
© Jin et al; licensee Springer. 2012
- Received: 9 September 2011
- Accepted: 2 February 2012
- Published: 2 February 2012
For high solar conversion efficiency of dye-sensitized solar cells [DSSCs], TiO2 nanofiber [TN] and Ag-doped TiO2 nanofiber [ATN] have been extended to be included in TiO2 films to increase the amount of dye loading for a higher short-circuit current. The ATN was used on affected DSSCs to increase the open circuit voltage. This process had enhanced the exit in dye molecules which were rapidly split into electrons, and the DSSCs with ATN stop the recombination of the electronic process. The conversion efficiency of TiO2 photoelectrode-based DSSCs was 4.74%; it was increased to 6.13% after adding 5 wt.% ATN into TiO2 films. The electron lifetime of DSSCs with ATN increased from 0.29 to 0.34 s and that electron recombination was reduced.
- dye-sensitized solar cell
- solar conversion efficiency
Since the Grätzel group discovered dye-sensitized solar cells [DSSCs], many people became interested. The low-cost, high-solar conversion efficiency of DSSCs is considered as a possible alternative to the present silicon solar cells [1–3]. DSSCs employ a sensitizer (dye) adsorbed on a surface of a wide energy bandgap semiconductor and electrolyte dissolving redox couples such as I-/I3- and platinum [Pt] counter electrode . In DSSCs, the photoexcited electrons of the dye adsorbing on the TiO2 surface are transferred to the conduction band of TiO2, which are then taken to an outer circuit using a fluorine-doped tin oxide [FTO] substrate and a counter electrode, respectively, and then the electrons are passed to an electrolyte [5, 6]. So, in order to get a high solar conversion efficiency in DSSCs, a high surface area for the porous TiO2 films for efficient absorption of the sensitizer and good networking between the particle to particle or particle to FTO substrate are very important [7–10]. So far, the TiO2-based DSSCs fabricated using multilayer approaches have shown the solar conversion efficiency of 11.3%, which is lower than the theoretical maximum (33%) [11, 12]. So many research, in order to increase the solar conversion efficiency in DSSCs, have been studied about photoelectrodes such as synthesis of the wide bandgap of TiO2, the small particle size of 10 to approximately 20 nm, the wide surface area of TiO2, and the porosity. As stated above, these can increase the adsorption of dye, and by extension, the solar conversion efficiency could be increased [13, 14].
In this study, DSSCs fabricated with a TiO2 nanofiber [TN] and an Ag-doped TiO2 nanofiber [ATN] were used to increase the TiO2 film's surface area for dye adsorption. The study has discussed the electrochemical properties of the TN-added cells or the ATN-added cells by photocurrent-voltage curves.
Preparation of TN and ATN
TN was fabricated using the electrospinning technique . The electrospinning technique has been recognized as a versatile and effective method for the production of fibers with small diameters and with high surface-to-volume ratio [16–18]. It is demonstrated that titanium isopropoxide [TiP] can be added directly to an alcohol solution containing polyvinylpyrrolidone [PVP] (with a molecular weight [MW] of 1,300,000). To suppress the hydrolysis reaction of the sol-gel precursor, acetic acid as well as PVP solution in ethanol must be added. TiP of 6 mL was mixed with 12 mL acetic acid and 12 mL ethanol. After 60 min, this solution was added to 30 g ethanol that contained 10 wt.% PVP and 1.986 mL of 0.5-N AgNO3 (5% TiP mol), followed by magnetic stirring for 24 h. The spinning solution underwent electrospinning with an applied voltage of 20 kV, a flow rate of 50 μL/min, and a tip to collector distance of 15 cm. The prepared electrospun fiber was calcinated at 500°C.
Preparation of the TiO2 photoelectrode and the Pt electrode
TiO2 paste was prepared by mixing nitric acid-treated and nanosized TiO2 (P-25, Degussa, Evonik Industries, Essen, Germany) powder with acetyl acetone, nitric acid, ethanol, distilled water, Triton X-100, and polyethylene glycol (Junsei Chemical Co., Ltd., Chuo-ku, Tokyo, Japan; average MW 20,000) binders for 10 h at 300 rpm by using the Planetary Mono Mill (pulverisette 6, Fritsch GmbH, Idar-Oberstein, Germany). In this process, the TiO2 powder was treated with nitric acid. The 12-g TiO2 (P-25) powder was mixed with distilled water and nitric acid (v/v, 120:1) at 80°C for 8 h using a hot plate. After mixing, the TiO2 nitric acid solution was dried at 100°C for 24 h. The prepared TiO2 paste was cast on pre-cleaned FTO (Pilkington FTO glass, Nippon Sheet Glass Co., Ltd., Minato-ku, Tokyo, Japan; 8 Ω/cm2) using the squeeze printing method. The coated TiO2 films were sintered at 450°C for 30 min. The active area of the TiO2 film was 0.25 cm2. The TiO2 film was immersed into a 5 × 10-4-mol/L ethanol solution of Ru(dcbpy)2(NCS)2 (535-bis, Solaronix Co., Aubonne, Switzerland) overnight, then rinsed with anhydrous ethanol, and finally dried. The counter electrode was prepared using the squeeze printing technique and subsequently sintered at 450°C for 30 min. The counter electrode material was a Pt catalyst (Solaronix Co.).
Assembly of the testing cells
The Pt electrode was placed over the dye-adsorbed TiO2 electrode, and the edges of the cell were sealed. The sealing was accomplished by hot-pressing two electrodes together at 120°C. The redox electrolyte was injected into the cell through two small holes drilled in the counter electrode. The redox electrolyte was composed of 0.3 mol/L 1,2-dimethyl-3-propylimidazolium iodide (Sigma-Aldrich Corporation, St. Louis, MO, USA), 0.5 mol/L 4-tert-butylpyridine (Sigma-Aldrich Corporation), and 3-metoxypropionitrile as solvent. The holes were then covered and sealed with a small square of sealing material and microscope objective glass.
The crystalline phase of the prepared TN and ATN was obtained by high resolution X-ray diffractometry [XRD] (D/MAX Ultima III, Rigaku Corporation, Tokyo, Japan) using CuKα radiation, and field-emission scanning electron microscopy [FE-SEM] (S-4700, Hitachi High-Tech, Minato-ku, Tokyo, Japan) and energy dispersive X-ray spectrometry [EDX] (EMAX Energy EX-200, HORIBA Ltd., Minami-Ku, Kyoto, Japan) were used to examine the morphology and chemical element analysis of the TiO2 film.
In order to investigate the physical and optical characteristics of the natural dyes, the UV-visible spectrum measurement was performed. The photovoltaic properties were investigated by measuring the photocurrent-voltage characteristics under illumination with an air mass [AM] of 1.5 (100 mW/cm2) simulated sunlight. The charge transport characteristics were investigated by intensity-modulated photovoltage spectroscopy [IMVS]. The IMVS was measured using red light-emitting diodes [LED] (635 nm). The light intensities were modulated by 10% in a frequency range typically from 0.01 to 100 Hz.
EDX data of pure TiO2 films and TiO2 films with 5 wt
(total = 100)
5 wt.% TN
(total = 100)
5 wt.% ATN
(total = 100)
In conclusion, TN and ATN were added into the TiO2 film of DSSCs. An enhanced η of 129% was achieved from the 5 wt.% ATN concentration. The added ATN had also contributed toward the enhancement of dye adsorption as seen from EDX results, and surface area was increased by the fibers. It gives many absorption sites for the dye, and the ATN that was added to the TiO2 film enhanced the charge recombination. The study has shown that the performance of DSSCs can be strongly improved using fibers. An η of approximately 6.13% has been achieved for DSSCs with ATN at the irradiation condition of AM 1.5 (100 mW/cm2) simulated sunlight, and Jsc, Voc, and FF are 14.93 mA/cm2, 0.68 V, and 60%, respectively. It is understood that the lifetime of DSSCs was increased by the addition of the ATN and that electron recombination was reduced.
This research was financially supported by the Ministry of Education, Science and Technology (MEST) and Korea Industrial Technology Foundation (KOTEF) through the Human Resource Training Project for Regional Innovation.
- Jeong J-A, Kim H-K: Thickness effect of RF sputtered TiO2passivating layer on the performance of dye-sensitized solar cells. Solar Energy Mater Solar Cells 2011, 95: 344–348. 10.1016/j.solmat.2010.02.008View ArticleGoogle Scholar
- Umar A: Growth of comb-like ZnO nanostructures for dye-sensitized solar cells applications. Nanoscale Res Lett 2009, 4: 1004–1008. 10.1007/s11671-009-9353-3View ArticleGoogle Scholar
- Lee SJ, Cho IH, Kim H, Hong SJ, Lee HY: Microstructure characterization of TiO2photoelectrodes for dye sensitized solar cell using statistical design of experiments. Trans Electr Electron Mater 2009, 10: 177–181. 10.4313/TEEM.2009.10.5.177View ArticleGoogle Scholar
- Jin EM, Park K-H, Jin B, Yun J-J, Gu H-B: Photosensitization of nanoporous TiO2films with natural dye. Phys Scr T 2010, 139: 014006.View ArticleGoogle Scholar
- Jung Y-S, Priya ARS, Lim MK, Lee SY, Kim K-J: Influence of amylopectin in dimethylsulfoxide on the improved performance of dye-sensitized solar cells. J Photochem Photobiol A: Chem 2010, 209: 174–180. 10.1016/j.jphotochem.2009.11.011View ArticleGoogle Scholar
- Lee K-M, Hu C-W, Chen H-W, Ho K-C: Incorporating carbon nanotube in a low-temperature fabrication process for dye-sensitized TiO2solar cells. Solar Energy Mater Solar Cells 2008, 92: 1628–1633. 10.1016/j.solmat.2008.07.012View ArticleGoogle Scholar
- Park K-H, Jin EM, Gu HB, Shim SE, Hong CK: Effects of HNO3treatment of TiO2nanoparticles on the photovoltaic properties of dye-sensitized solar cells. Mater Lett 2009, 63: 2208–2211. 10.1016/j.matlet.2009.07.034View ArticleGoogle Scholar
- Jin EM, Park K-H, Yun J-J, Hong CK, Hwang M-J, Park B-K, Kimm K-W, Gu H-B: Photovoltaic properties of TiO2photoelectrtode prepared by using liquid PEG-EEM binder. Surface Rev Lett 2010, 17: 15–20. 10.1142/S0218625X10013576View ArticleGoogle Scholar
- Horea S, Vetter C, Kerna R, Smit H, Hinsch A: Influence of scattering layers on efficiency of dye-sensitized solar cells. Solar Energy Mater Solar Cells 2006, 90: 1176–1188. 10.1016/j.solmat.2005.07.002View ArticleGoogle Scholar
- Ko KH, Lee YC, Jung YJ: Enhanced efficiency of dye-sensitized TiO2solar cells (DSSC) by doping of metal ions. J Colloid Interface Sci 2005, 283: 482–487. 10.1016/j.jcis.2004.09.009View ArticleGoogle Scholar
- Fuke N, Fukui A, Islam A, Komiya R, Yamanaka R, Harima H, Han L: Influence of TiO2/electrode interface on electron transport properties in back contact dye-sensitized solar cells. Solar Energy Mater Solar Cells 2009, 93: 720–724. 10.1016/j.solmat.2008.09.037View ArticleGoogle Scholar
- Xu C, Shin P, Cao L, Wu J, Gao D: Ordered TiO2nanotube arrays on transparent conductive oxide for dye-sensitized solar cells. Chem Mater 2010, 22: 143–148. 10.1021/cm9027513View ArticleGoogle Scholar
- Tang Y-B, Lee C-S, Xu J, Liu Z-T, Chen Z-H, He Z, Cao Y-L, Yuan G, Song H, Chen L, Luo L, Cheng H-M, Zhang W-J, Bello I, Lee S-T: Incorporation of graphenes in nanostructured TiO2films via molecular grafting for dye-sensitized solar cell application. Am Chem Soc 2010, 4: 3482–3488.Google Scholar
- Nair AS, Jose R, Yang S, Ramasrishna S: A simple recipe for an efficient TiO2 nanofiber-based dye-sensitized solar cell. J Colloid Interface Sci 2011, 353: 39–45. 10.1016/j.jcis.2010.09.042View ArticleGoogle Scholar
- Park JY, Lee IH, Bea GN: Optimization of the electrospinning conditions for preparation of nano fibers from polyvinylacetate (PVAc) in ethanol solvent. J Ind Eng Chem 2008, 14: 707–713. 10.1016/j.jiec.2008.03.006View ArticleGoogle Scholar
- Park JY, Lee I-H: Characterization and morphology of prepared titanium dioxide nanofibers by electrospinning. J Nanosci Nanotechnol 2010, 10: 3402–3405. 10.1166/jnn.2010.2300View ArticleGoogle Scholar
- Li D, Xia Y: Fabrication of titania nanofibers by electrospinning. Nano Lett 2003, 3: 555–560. 10.1021/nl034039oView ArticleGoogle Scholar
- Ding B, Kim H, Kim C, Khil M, Park S: Preparation and characterization of nanoscaled poly(vinyl alcohol) fibers via electrospinning. Nanotechnol 2003, 14: 532–537. 10.1088/0957-4484/14/5/309View ArticleGoogle Scholar
- Park JY, Yun J-J, Hwang C-H, Lee I-H: Influence of silver doping on the phase transformation and crystallite growth of electrospun TiO2nanofibers. Mater Lett 2010, 64: 2692–2695. 10.1016/j.matlet.2010.09.008View ArticleGoogle Scholar
- Spurr RA, Myers H: Quantitative analysis of anatase-rutile mixtures with an X-ray diffractometer. Anal Chem 1957, 29: 760–762. 10.1021/ac60125a006View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.